Compression molding is a method of molding in which the molding material, generally preheated, is first placed in an open, heated mold cavity. The mold is closed with a top force or plug member, pressure is applied to force the material into contact with all mold areas, while heat and pressure are maintained until the molding material has cured. The process employs thermosetting resins in a partially cured stage, either in the form of granules, putty-like masses, or preforms. Compression molding is a high-volume, high-pressure method suitable for molding complex, high-strength fiberglass reinforcements. Advanced composite thermoplastics can also be compression molded with unidirectional tapes, woven fabrics, randomly oriented fiber mat or chopped strand. The advantage of compression molding is its ability to mold large, fairly intricate parts. Also, it is one of the lowest cost molding methods compared with other methods such as transfer molding and injection molding; moreover it wastes relatively little material, giving it an advantage when working with expensive compounds. However, compression molding often provides poor product consistency and difficulty in controlling flashing, and it is not suitable for some types of parts. Fewer knit lines are produced and a smaller amount of fiber-length degradation is noticeable when compared to injection molding. Compression-molding is also suitable for ultra-large basic shape production in sizes beyond the capacity of extrusion techniques. Materials that are typically manufactured through compression molding include: Polyester fiberglass resin systems (SMC/BMC), Torlon, Vespel, Poly(p-phenylene sulfide) (PPS), and many grades of PEEK.
Compression molding was first developed to manufacture composite parts for metal replacement applications, compression molding is typically used to make larger flat or moderately curved parts. This method of molding is greatly used in manufacturing automotive parts such as hoods, fenders, scoops, spoilers, as well as smaller more intricate parts. The material to be molded is positioned in the mold cavity and the heated platens are closed by a hydraulic ram. Bulk molding compound (BMC) or sheet molding compound (SMC), are conformed to the mold form by the applied pressure and heated until the curing reaction occurs. SMC feed material usually is cut to conform to the surface area of the mold. The mold is then cooled and the part removed. Materials may be loaded into the mold either in the form of pellets or sheet, or the mold may be loaded from a plasticating extruder. Materials are heated above their melting points, formed and cooled. The more evenly the feed material is distributed over the mold surface, the less flow orientation occurs during the compression stage.
Thermoplastic matrices are commonplace in mass production industries e.g. automotive applications where the leading technologies are Long Fibre reinforced Thermoplastics (LFT) and Glass fiber Mat reinforced Thermoplastics (GMT).
In compression molding there are six important considerations that an engineer should bear in mind:
- Determining the proper amount of material.
- Determining the minimum amount of energy required to heat the material.
- Determining the minimum time required to heat the material.
- Determining the appropriate heating technique.
- Predicting the required force, to ensure that shot attains the proper shape.
- Designing the mold for rapid cooling after the material has been compressed into the mold.
Other articles related to "molding, compression molding":
... Transfer molding, ( BrE moulding ) like compression molding, is a process where the amount of molding material (usually a thermoset plastic) is measured and ... The molding material is preheated and loaded into a chamber known as the pot ... Transfer Molding ...
... A quicker method uses a compression mold ... This is a two-piece (male and female) mold usually made out of fiberglass or aluminum that is bolted together with the fabric and resin between the two ...
Famous quotes containing the words molding and/or compression:
“To translate, one must have a style of his own, for otherwise the translation will have no rhythm or nuance, which come from the process of artistically thinking through and molding the sentences; they cannot be reconstituted by piecemeal imitation. The problem of translation is to retreat to a simpler tenor of ones own style and creatively adjust this to ones author.”
—Paul Goodman (19111972)
“The triumphs of peace have been in some proximity to war. Whilst the hand was still familiar with the sword-hilt, whilst the habits of the camp were still visible in the port and complexion of the gentleman, his intellectual power culminated; the compression and tension of these stern conditions is a training for the finest and softest arts, and can rarely be compensated in tranquil times, except by some analogous vigor drawn from occupations as hardy as war.”
—Ralph Waldo Emerson (18031882)